shrinkage-compensating concretes for special structures shrinkage-compensating concretes can be...
Post on 02-Jun-2020
Embed Size (px)
SHRINKAGE-COMPENSATING CONCRETES FOR SPECIAL STRUCTURES
Roberto Troli and Mario Collepardi
Shrinkage-compensating concretes have been extensively used in the last forty years to minimize cracking caused by drying shrinkage in reinforced concrete structures.
The first and most diffused system to produce shrinkage-compensating concretes involves the use of expansive cements, according to ACI 223-98, instead of ordinary portland cement. All these special binders are based on a controlled production of ettringite.
Another effective method to produce shrinkage-compensating concretes, not covered by ACI 223-98 but commonly used in some countries, like Italy or Japan, lies in the use of a CaO and/or MgO based expansive agent. This technology seems to be more advantageous with respect to that based on the ettringite formation from an economical as well as from a practical point of view.
Recently, the addition of a shrinkage-reducing admixture (SRA) has been found to improve the behavior of CaO based shrinkage-compensating concretes especially in the absence of an adequate wet curing.
Although the actual cause of this synergistic effect has not been completely explained, the use of this technology in construction industry has been increased, in the last five years, particularly in Italy, with very interesting results.
In this work three remarkable examples of special reinforced concrete structures are presented in which the use of CaO-SRA based shrinkage-compensating concretes was successfully carried out in order to prevent shrinkage related cracks and/or joints excessive opening in the presence of adverse curing conditions which are normally not suitable for the use of this technique.
1 Shrinkage and Shrinkage related cracks
Drying shrinkage is a volume contraction which occurs in the concrete during hardening, caused by moisture loss. If drying shrinkage could take place freely, without any restraint, it wouldn’t represent any problem for most structural and non-structural concrete elements. Unfortunately, because of the presence of internal and external restraints (steel reinforcement, linkage with other portions of the structure, subgrade friction in slab on grade, etc.) drying contraction is partially, or totally, hindered and transformed in tensile stresses.
While concrete is a brittle material, drying shrinkage stresses are often large enough to exceed the tensile strength of the concrete, resulting in cracks formation.
Drying shrinkage cracks represent one of the main problems affecting reinforced concrete structures and elements since they are often cause of early deterioration, loss of serviceability or, simply, aesthetic defects formation.
Actually, the formation of cracks nullifies the adoption of a potentially impermeable, low w/c concrete in assuring the required durability of reinforced concrete structures which are exposed to
environmental aggressive agents such as carbonation and chlorides since steel rebars are immediately subjected to corrosion.
Cracks due to drying shrinkage may compromise the serviceability of concrete pavements subjected to heavy traffic loads or special marine or hydraulic constructions which must assure watertightness.
Finally, cracks may represent a concern even if they compromise the aesthetic aspect of not exposed architectural concrete structures.
2 Shrinkage-Compensating Concretes
Probably the use of shrinkage-compensating concretes is the most effective method to eliminate or, at least, minimize, the formation of drying shrinkage related cracks in reinforced concrete structures.
This technique is based on a volume expansion which is induced in the concrete by a specific chemical reaction whose effects can be adequately designed and controlled by the correct proportioning of the concrete.
Normally the induced chemical expansion occurs during the first 2-7 days being so much faster than the contractions caused by moisture loss. For this reason, in order to be advantageously used to compensate drying shrinkage, the early expansion must be adequately restrained by a proper design and location of the steel deformed bars and/or by other means of restraint.
In this way, an early compressive stress is induced in the concrete which will compensate for tensile stresses caused by the subsequent restrained drying shrinkage.
According to the ASTM C 878 test method , the expansive behavior of a shrinkage- compensating concrete is determined by measuring the length change of a steel rebar embedded in concrete prismatic specimens, demoulded at the setting time (about 6-8 hours after mixing) and kept under lime-saturated water for 7 days.
To provide satisfactory shrinkage compensation, the required expansion in the reinforced structural member is recommended to be greater than, or at least equal to, the predicted shrinkage in the member.
According to ACI 223-98 , the design of a shrinkage compensated reinforced concrete member must include the four following steps.
a) Estimation of member shrinkage. First of all, a sufficiently reliable prediction of the member final drying shrinkage must be carried out. In this estimation, the effects of member thickness, reinforced amount, relative humidity, concrete composition and type of aggregate must be taken into account.
b) Selection of the required member expansion. According to ACI 223R, to provide satisfactory shrinkage compensation, the required expansion in the reinforced structural member is recommended to be greater than, or at least equal to, the anticipated shrinkage. This required expansion may be greater than that strictly necessary to offset drying shrinkage if remarkable thermal contractions during service life are expected and need to be compensated.
c) Estimation of specimen expansion: The ASTM C 878 specimen expansion which is necessary to provide the required member expansion can be easily obtained by using the graph shown in Figure 1, taken from ACI 223-98 and based on data published by Russell
in 1973). The graph gives the relation between member expansion and specimen expansion as a function of actual percentage of reinforcement in the designed member;
d) Proportioning of shrinkage-compensating concrete in order to assure the calculated specimen expansion.
The early chemical expansion induces tensile stresses in steel reinforcement. These stresses are generally lower than that allowed for the material if the requirements of ACI 318 (or those of equivalent codes in force in other countries, such as the eurocodes in the European Community) are satisfied. Furthermore, these stresses are normally destined to disappear with time as shrinkage goes on.
Sometimes, in the case of early heavy loaded structures, the tensile stresses caused by expansion must be considered, in addition to those induced by external loads, in order to verify structural safety. For the same reason, the initial compressive stresses induced in the concrete by the restrained expansion must be added to those caused by eventual early external loads in order to provide proper safety factors in the first period of the service life of the structure. These additional compressive stresses in concrete can be easily determined, as a function of reinforcement percentage and member expansion, by using the graph of Figure 2 (ACI 223-98).
Figure 1 – Member expansion as a function of ASTM C 878 specimen expansion (ACI 223-98)
Figure 2 – Concrete compressive stress induced by member restrained expansion (ACI 223R-98)
3 Expansive Cementis
Shrinkage-compensating concretes can be manufactured by using special expansive cements instead of normal portland cement.
The first examples of expansive cements were developed in Russia and in France. In particular, in the early 40th of the previous century Lossier  realized an expansive cement by mixing an ordinary portland cement with an expansive agent, based on calcium sulphate and calcium aluminates, and a stabilizer consisting in blast furnace slag.
The expansion was given by the reaction between calcium sulphate, calcium aluminates and water to form ettringite. The control of the expansion was delegated to the blast furnace slag which gradually substituted calcium aluminates in the reaction with calcium sulphate bringing it to an end. In the following years several expansive cements were ideated most of all based on a controlled production of ettringite.
ASTM C845-90 and ACI 223-98 classify the following three different types of expansive cements: 1) type K (Klein cement), containing C4A3S1, calcium sulphate (CaSO4) and free CaO; 2) type M, produced by blending portland cement with calcium aluminates CA1 and C7A121; 3) type S, which contains excess of C3A1 and CS1 with respect to that usually found in portland
Among the above listed expansive cements, the most diffused is the type K which can be alternately produced by intergrinding portland cement with a separately burned expansive component or simultaneously burning all components to obtain an expansive clinker.
The expansive reaction which takes place in both cases can be represented as follows1:
C4A3S + 6C + 8 CS + 96 H → 3(C3A⋅3CS⋅32H) (1)
1 Cement chemistry contracted symbology: C = CaO, A = Al2O3, S = SiO2, H = H2O a